A review of physical experimental research in jet electrochemical machining
- 142 Downloads
Jet electrochemical machining (Jet-ECM) is a non-traditional machining process that has developed rapidly since its introduction in the 1980s with progress being made in micro-machining and surface finishing. This paper critically reviews the development of physical experimental work in Jet-ECM and corresponding hybrid technologies and their applications, e.g. laser- and air-assisted Jet-ECM. In addition to discussing the merits of the physical experimental research, the paper concludes with research challenges in the future of Jet-ECM development.
KeywordsAir-assisted Jet-ECM Electrochemical machining Jet electrochemical machining Laser-assisted Jet-ECM
Jet-ECM, also known as electro jet drilling, electro jet machining, electrochemical jet machining is a non-traditional machining technique in which a free jet of electrolyte locally removes material from an electrically conductive workpiece via anodic dissolution. Although Jet-ECM is developed from and shares several similarities with traditional electrochemical machining (ECM), it has its own unique characteristics. Unlike ECM, jet-ECM does not use a tool to produce a negative imprint in the workpiece; instead, a pressurised jet of electrolyte is expelled through a nozzle to locally dissolve material at the contact area between the jet and the workpiece .
Although the concept of Jet-ECM first appeared in the 1980s , the rate of research and development has accelerated in the twenty-first century, both in physical experimentation and in modelling and simulation of the process, for example, simulation of material removal  and energy distribution modulation . Jet-ECM has become an attractive area of research due to its benefits over both traditional and alternative electrochemical processes due to its ability to machine micro-size features regardless of material hardness, without producing heat-affected zones, surface stresses, micro cracks and burrs at good energy efficiency . These characteristics lend Jet-ECM to several manufacturing sectors, including but not exclusive to aerospace, micro-electronics, medical and biomedical applications.
This paper critically reviews the development of physical experimental work in Jet-ECM and corresponding hybrid technologies and their applications, that is experimental work exclusive of modelling and simulation studies.
2 Overview of the Jet-ECM process
In the case of Jet-ECM, the electronically conductive workpiece becomes the anode, and the nozzle the cathode.
The dissolution process continues in this continuous cycle. However, as previously mentioned, there are several dissolution mechanisms and variables. For example, in oxygenated environments, the ionic metal can react with the oxygen to produce new oxide layers on the material surface which in turn have to be overcome. Due to this process occurring only at areas on the workpiece in contact with the electrolyte jet, the electrochemical reaction provides localised and controlled material removal. When material removal rates and profiles are known with controlled process parameters, Jet-ECM has the ability to machine micro features.
3 Unassisted Jet-ECM
The majority of research performed in the field of jet-ECM has been physical experimentation, and within that bracket most has been performed in unassisted Jet-ECM, that being using only an electrolyte jet with no laser  or ultrasonic assistance .
- k 0
= measured conductivity at 180C
- Δ T
= difference in temperature from 18 ∘C
- f(Δ T)
= polynomial function of Δ T
The authors also focus on the relationship between the working parameters (nozzle diameter, electrolyte flow rate, voltage and gap) and the diameter of the hole produced at these parameters. It was found that the ratio of the diameter of the hole to the nozzle has a minimum value that decreases with voltage and at an optimum flow rate for each voltage. It was concluded that the ratio could never be nominal, that there is ‘no simple relationship between the working parameters and the hole diameters’  and that working gap had no influence on the hole diameter.
Parameters for best hole quality 
Capillary outside diameter
Inlet electrolyte pressure
At constant current, pit depth vs. time is a positive linear relationship, but surface roughness does not vary with time.
Increase in current improves surface roughness values, up to a current density (J) of 110 A/cm2 where the relationship plateaus.
When machining grooves, lower speeds produce higher removal, while surface finish is improved with more scanning runs due to reduced exposure to the peripheral low current density.
In 2011, Kunieda et al. proposed a novel technique for Jet-ECM. Whereas earlier Jet-ECM experimentation was developed around the use of a cylindrical nozzle, the use of an elongated or ‘letter box’–shaped nozzle was first used in order to increase the jet contact area . An investigation into jet quality showed that the working gap plays a big role. The length of the machined profile, parallel to the slit nozzle decreased with increased gap, but the width increased. Increasing the pressure caused the jet to keep better shape, but the ends of the produced groove were rounded due to surface tension at the jet edges, an issue not found with traversing cylindrical nozzles. An expanding throat nozzle was introduced to combat the larger width at larger working gaps. Expanding the jet parallel to the slit direction allows the thickness to decrease. The machined groove length increased with increasing working gap up to 6.5 mm; where it began do decrease due to surface tension with increased working gap.
In setting up a new generator to an existing Jet-ECM prototype, Schubert  studied the influence of electrical voltage and working gap on achieved current densities and widths, depths and surface qualities of the machined geometries. Although several of these relationships had been studied before, for example current and surface roughness relationships , this experiment includes preliminary studies to specify breakdown voltages at several working distances, allowing a safety against breakdown and derivation of maximum working voltages at each distance. At working distances below 20 μ m, wide and imprecise cavities were generated, up to 2.5 times the nozzle diameter. This was due to the fact that in such a short gap, a free jet is unable to form and the nozzle is in fact enclosed by the electrolyte .
Over a range of 5–100 V and working gaps of 10–100 μ m, higher voltages produced higher material removal rates, and larger working gaps reduced material removal; however as previously mentioned, at small working gaps, accuracy is reduced. Schubert  found that surface roughness values improve with increased current, the same trend found by Natsu et al. . The surface roughness value of 0.1 μ m Rz achieved by Schubert is an improvement on that achieved by Natsu et al. As expected, applied current decreases with distance at constant voltage due to increased resistance over the length of the jet, while at constant working distance, applied current increases with voltage.
Kawanaka et al. also compare the influence of electrolyte on surface textures. At low current densities, complicated porous structures were produced, but within that, sodium chloride produced larger pores than the sodium nitrate counterpart showing that the surface morphology is electrolyte dependant and surface textures can be varied by changing electrolyte and current densities .
Later, Kawanaka and Kunieda investigated the effect of translating speed on surface roughness, as well as producing a comparison between finishing with direct current, pulse current and bipolar pulse current . To study the effect of translating speed on surface roughness, the number of reciprocating translations changed in proportion to translated speed and inversely proportional to current density to machine grooves of the same depth. It was found that increasing translational speeds produced better surface finishes at all current densities studied, with all current densities being above the threshold value for machining.
In an electrolyte jet, the current distribution causes the current density to be higher at the centre of the jet than on the outer edges. While the high current density smooths the surface quickly, the lower current densities roughen the surface in comparison [10, 15] and at lower translating speeds, the dwell time over a certain point causes a roughing effect. However at higher translational speeds, this roughing effect becomes insignificant as the dwelling time is short .
Furthermore, when comparing the surface roughness without translation and with translation of 100 mm/s, only one current density investigated had a better surface roughness value without translation, leading to a belief that producing mirror surfaces requires translation as a prerequisite . However, mirror surfaces (< 0.2 μ m Ra) were achieved when pitting in a previous paper , therefore, although translating speeds aid surface roughness, it is not a prerequisite, especially in machining situations where high-speed translation is difficult or not required. Although built upon the previous study by Kawanaka et al. , the surface roughness values of 14.1 nm Ra were not re-iterated in this study.
Chen et al.  proposed a method of machining micro dimples through the use of a conductive mask. The use of a conductive mask was thought to reduce the intensity of the electric field around the edge of the dimple. The mask used had through holes of 200 μ m diameter on stainless-steel samples. The machining localisation was improved with the use of a conductive mask over an insulated mask, at the cost of a reduction in current efficiency . Comparatively, this study produced dimples 240 μ m wide by 85 μ m deep, no better than those achieved by Hackert-Oschätzchen et al.  without the use of a mask. It is worth noting that the mask requires close contact with the surface, so limits the method to flat surfaces. Although the conductive mask presents benefits over traditional Jet-ECM, the inclusion removes a benefit of the process over traditional manufacturing and EDM in the need for no specific tooling.
Similarly to the studies on electrolyte jet turning performed by Kunieda et al.  and Mizugai et al. , Martin et al. analysed the removal geometries in Jet-ECM profile turning . Unlike the previous studies by Kunieda et al.  and Mizugai et al.  in which a ‘letter box’ nozzle was used, Martin et al. performed the turning operations with a cylindrical jet . Voltages of 10 to 60 V were analysed with the number of rotations increased from a single rotation to 10 rotations at constant rotational speed for each voltage. It was found that removal depth increased with both increased voltage and increased rotations in a non-linear fashion, with a declining increase with increased rotations at all voltages, attributed to increased resistance with increased IEG. In a comparison with Jet-ECM on planar surfaces, the width of channels was lower in the turning application at similar removal depths to those on planar surfaces .
Whereas Jet-ECM is usually performed in an unsubmerged environment, Ming et al. studied the Jet-ECM process in a kerosene submerged environment . They expected that submerging the process in an insulating liquid medium would enhance the localization of the current in the jet. It was found at all applied voltages; surface roughness was improved in the submerged experiments in comparison with an unsubmerged experiment. However, improvement of localisation, or aspect ratio of dimples, was only found at specific parameters, namely at lower applied voltages. For example, at a working gap of 0.2 mm, aspect ratio was only improved at applied voltages lower than 14 V . Although at some parameters kerosene submerging provides a benefit over standard jet-ECM, in general, no improvement is seen or dimple diameters are larger with kerosene submersion. Kerosene submersion adds an extra complexity to the process, as well as safety concerns.
Up to this point, all mentioned experimental studies have been performed on stainless-steel workpieces of various kinds. The rest of this section addresses experimentation performed on other materials and the variations in processes and results that arise.
Lu and Leng performed a study into the use of Jet-ECM on titanium alloy (Ti6Al4V) surfaces for biomedical applications where surface features in the range of 100 μ m are essential on load-bearing implants . They used a metal nozzle of diameter 300 μ m coated in epoxy to reduce the electrical resistance and an electrolyte of 5 mol/L NaBr aqeous solution. In general, the current density used in this study was low compared with previous studies with values less than 50 A/cm2; however, the depths of machined holes in the study were greater than 1 mm after 3 min of machining, with a depth to width ratio of between 1.2 and 1.4 and the diameters of the holes produced being over two times the diameter of the nozzle. When compared with through mask ECM, although through mask ECM produces regular patterns in a batch process, the Jet-ECM process can be used on irregular curved surfaces, and produce holes with a higher aspect ratio with a more simple setup .
Secondary findings show that increasing the salt factor of the electrolyte (increasing the conductivity by a factor of 1.5) increases the aspect ratio of machined pits, as seen previously, longer machining times increased both the width and depth of machined pits, and again, opposing Ippolito et al.  increasing the gap width results in wider profiles up to an optimal electric potential . Overall, the surface roughness was not improved over the original ground surface, as the grain size is the predominant factor in the surface roughness of the material.
An alternative study for Jet-ECM of cemented carbides was presented by Mizugai et al. in the same year . Whereas Hackert-Oschätzchen et al.  were unable to machine tungsten carbide with a pH-neutral sodium nitrate solution, Mizugai et al. successfully performed this task using both D.C. and A.C. currents. Mizugai et al. found that NaOH was formed at the cathode during the Jet-ECM process, and is in turn transferred to the anodic workpiece via the electrolyte jet flow, meaning no NaOH had to be added to the original electrolyte. However, the NaOH is produced on the inner wall of the nozzle, and is therefore transferred in the outer areas of the jet, causing wider machined geometries (4 times the nozzle diameter) as the NaOH required to breakdown the material is not mixed to the centre of the nozzle .
Replacing the metallic nozzle with one made of ceramic allows premixing of the NaOH into the electrolyte in a metallic nozzle holder, and then applied to the workpiece equally to the workpiece. As the current is highest in the centre of the jet contact area, the ceramic nozzle allowed deeper, more precise machining under a direct current. This result was up to a current limit of 30 mA, as further increased current resulted in shallower, wider pits as the current limit for breakdown was reached over a wider area.
When using an A.C. current with ceramic nozzle, machined depth increased with current and time, up to a limit where the pit depth became saturated if the current was too high. The optimum current frequency was found to be 5 Hz, and duty factor of 70%. At a lower duty factor, surface roughness increased, above 70%, the pit shape became erratic .
In 2016, Hackert-Oschätzchen et al. studied the machining of particle-reinforced aluminium matrix composites using both sodium nitrate and sodium chloride pH-neutral electrolytes . The experiments were performed on an EN AW 2017 aluminium matrix containing silicon carbide particles of either 5 or 10% content. Both electrolytes were used in quantities that provided the same conductivity of 185 mS/cm. They found that in preliminary testing, sodium nitrate produced a passivating effect on the aluminium surface, whereas sodium chloride did not, and also provided more rounded edges to the pit machined. At a machining voltage of 20 V and for a time of 2 s, using sodium chloride produced pits nearly twice as deep as that using sodium nitrate, where both had pit widths twice the nozzle diameter. In conjunction with other experiments studied in this paper, depth and width of machined pits increased with voltage and machining time. Interestingly, changing the percentage of silicon carbide particles in the matrix did not change the machining results .
Building upon the work performed by Kunieda et al. on electrochemical turning using a flat jet  and by Mizugai et al. on machining cemented carbide , Miyoshi and Kunieda developed a jet turning system for the machining of cemented tungsten carbide rods . As seen by Hackert-Oschätzchen et al.  and by Mizugai et al. , when machining with a DC current on tungsten carbide, a tungsten oxide layer was formed on the workpiece, preventing further machining. Using the bipolar current investigated by Masuzawa and Kimura  and using current parameters from the experiment by Muzugai et al. (5Hz at a 50% duty factor), Miyoshi and Kunieda achieved an aspect ratio of 20 on a turned section of a tungsten carbide rod, with a finished diameter of 36 μ m. However, contrary to the results of Hackert-Oschätzchen et al. , material removal increased with decreasing grain size, although the range of grain sizes was much larger in Miyoshi and Kunieda’s investigation (2-10 μ m) compared with 1–4 μ m in the Hackert-Oschätzchen et al.  study. It is also worth noting that the duty factor selected in this experiment is different to the optimum found by Mizugai et al.  of a 70% duty factor as although material removal is less at 50% duty factor, the width of the machined geometry is significantly reduced, allowing more accurate turning. Like Hackert-Oschätzchen et al. , Miyoshi and Kunieda did agree that the surface roughness values achieved are heavily influenced by the grain size .
Similarly to how Hackert-Oschätzchen et al.  studied the effect of electrolytes on an aluminium alloy, Speidel et al.  investigated the Jet-ECM of titanium alloys using novel electrolyte solutions, specifically how the use of bromides, chlorides and flourides compare with nitrates on surface finish, material removal rate and pit formation. It was known that during the ECM process, a non-conductive passivating layer formed on the material surface and that neutral pH electrolyte had previously performed poorly on titanium alloys.
Due to the insolubility of sodium fluoride in water, it could not be directly compared with the other electrolytes at the studied concentrations and therefore a sodium chloride electrolyte doped with fluoride was used for comparison . In agreement with Sen and Shan  when increasing the concentration of salt in the solution, the pit depth increased when using sodium nitrate. However, for the chloride- and bromide-based electrolytes, increasing the salt concentration had no effect on the machined depth achieved allowing similar machining performance to be achieved with lower electrolyte concentrations. The fluoride-doped electrolyte achieved lesser depths than the chloride-only electrolyte in the same concentration.
Liu et al. published a comprehensive study on machining TB6 titanium alloy with aiming for industrial applications . They used a copper nozzle of 2 mm diameter, much larger than those seen in previous experiments, for example 50 μ m  and 100 μ m ; however, the focus is based more upon material removal than the machining of microgeometries. Investigations included a large range of voltages, working gap and flow rate parameters in depth, and for the first time the effect of electrolyte temperature on machining results, although it had been previously touched upon by Natsu et al. . Liu et al. also give a more in-depth analysis on the effect of electrolytes and the associated mechanisms . Whereas previous studies analyse the surfaces machined using various electrolytes , they suggest the reason for the chloride-based electrolytes are more effective at machining titanium due to the ions being much smaller and more efficient at penetrating the oxide passive layer.
Increasing the sodium chloride electrolyte temperature from 20 to 60 ∘C halved the energy required to activate the dissolution process as at higher temperatures, the attack and removal of the passive layer are accelerated . However, Liu et al. found there to be a limiting factor to the temperatures used, as in the inter electrode gap (IEG), the electrolyte can increase in temperature by 60 ∘C and if evaporation occurs, performance is severely hindered. When using sodium nitrate, increased temperatures in the electrolyte increase the rate of oxidation making the surface more counterproductive for machining. When investigating parameters for material removal, in agreement with Speidel et al. , it was found that increasing the concentration of sodium chloride resulted in higher material removal on titanium due to higher conductivity and therefore higher current at constant voltage. In the research, it was found the same relationship as Schubert  in that increasing the inter electrode gap decreases the material removal rate as well as discovering an increased flow rate improves material removal rates .
Optimum parameters and machining results on TB6 titanium alloy 
Machining results using
Voltage: 24 V
Material removal rate: 10.062 g/min
IEG: 0.6 mm
Surface roughness: 0.231 μ m
Flow rate: 2.1 L/min
Electrolyte: NaCl 15%
Average overcut: 1.01 mm
It was found the off-centre single point element nozzle produced the deepest machined profile, and the symmetrical twin element nozzle produced a wider cut than the standard nozzle, but with steeper side walls . Overall, the study showed that altering the mechanical design of the nozzle can alter the profile of the machined areas in comparison with a standard nozzle, and that combinations of nozzles can machine complex geometries providing a larger degree of control and profile prediction.
Clare et al. purposely built an enhanced tool holding system to allow the nozzle angle to index relative to the workpiece . In the study, nozzle orientations of 22.5∘ and 90∘ were compared on Inconel 718 workpieces, with two current densities (200 and 400 A/cm2) and two nozzles, one standard and one chamfered similar to that in the study by Mitchell-Smith et al. . They found the use of an iodide-doped electrolyte increases the precision with a 172% increase in slope and 99% reduction in overcut compared with standard sodium nitrate electrolyte. The chamfered nozzle at 22.5∘ orientation significantly enhances the precision of the cut. Overall comparisons between modes, or combinations of electrolyte, nozzle and orientation angle are also analysed.
In a similar study to that of Clare et al. , Mitchell-Smith et al. also studied the effect of nozzle orientations on an Inconel 718 workpiece . Whereas Clare et al.  studied two nozzle orientations, Mitchell-Smith et al.  studied the effect of nozzle orientations of 22.5∘, 67.5∘ and 90∘ to the material surface, as well as the effect of machining direction relative to the nozzle orientation angle, which they define as ‘pushing’ or ‘pulling’ while varying the jet flow rate. It was found the surface finish was better when the nozzle was ‘pushed’ or angled towards the direction of movement compared with when the nozzle is angled away or ‘pulled’. This is due to the current being higher on the trailing edge of the jet due to a lower IEG, and the surface roughness is dominated by the parameters of the trailing edge, as this machines the surface last. Orientating the nozzle at 22.5∘ or 157.5∘ increased the depth of the machined profile by 23% in comparison with a 90∘ orientation. The jet velocity had no noticeable effect on the results in this study .
A study into the finishing of silicon carbide re-enforced aluminium using various electrolytes was produced by Lehnert et al. . The study looks into the use of sodium bromide, sodium chloride and sodium nitrate on finishing aluminium matrices of 0, 5 and 10% SiC particles under identical process parameters. It was found dissolution characteristics are electrolyte dependent, with sodium chloride electrolyte producing the deepest point erosions, and sodium nitrate electrolyte the shallowest, results in keeping with those produced by Hackert-Oschätzchen et al. . Similarly to Hackert-Oschätzchen et al. , the percentage of silicon carbide particles in the matrix did not affect machining using sodium nitrate electrolyte . However, with the use of sodium chloride, a larger percentage of particles reduced the width and depth of erosions, while using sodium bromide, the presence of particles reduced the width and depth of erosions, but is less influenced by the percentage of particles themselves.
Mitchell-Smith et al.  built upon a previous study of nozzle geometry, introducing sodium iodide (NaI)-doped electrolytes and including the concept of current filtering and re-fresh rate at varying machining parameters. Material removal associated with NaCl-, NaNO3- and NaI-doped electrolytes are compared and analysed. As in the study previous of nozzle geometry, the ability to machine complex surface structures with varying nozzles was illustrated. However, with the inclusion of the doped electrolyte, precision with the use of the complex nozzles is improved but at the cost of lower current efficiencies with increasingly doped electrolytes. Overall, dimensional accuracy improvements and ‘superior surface intersection’ are achieved with iodide-enhanced electrolytes; however, there is a decrease in material removal rates with increased doping .
Mitchell-Smith et al. aimed to build upon the work produced by Speidel et al.  to utilise the effects of different electrolytes for the optimisation of feature generation on an Inconel 718 workpiece . They produced a system capable of electrolyte multiplexing, with the ability to mix four separate electrolyte tanks. For this study, striations were produced with two passes over a coincident toolpath, using various combinations of the electrolytes. The electrolytes used were NaNO3, NaCl and NaI, or more specifically a mixed sodium nitrate and sodium iodide solution with 20% NaI referred to as NaI20 as previously used by Mitchell-Smith et al. , with all electrolytes kept at the same temperature and concentration. It was found the best combination took advantage of the high removal rate of NaCl followed by the better surface finish produced by NaI2O. The study shows the ability to combine both precision and material removal performance, as well as the ability to produce continuous profiles of varying surface properties .
Speidel et al.  showed that material precondition effects the resultant surface produced by Jet-ECM when comparing an annealed and non-annealed copper sheet. They found for fine-grained materials, surfaces are more porous post-machining at lower current densities than those that have been annealed and are therefore large grained. Increasing the current density overcomes any pre-existing grain texture, as well as reducing pore size.
4 Assisted Jet-ECM
Assisted jet-ECM is the combination of jet-ECM with additional technologies to produce a hybrid system. The aim of these hybrid systems is to improve at least one area of the unwanted machining characteristics in Jet-ECM such as overcutting, stray machining, tapered holes and aiming to improve the performance and capability of the process [37, 38].
4.1 Laser-assisted Jet-ECM
Laser-assisted Jet-ECM (LAJECM) is the combination of a low power laser working co-axially with the electrolyte jet to improve the process localisation by heating both the electrolyte jet and the workpiece surface at the centre of the contact with the jet. The thermal energy of the laser transmitted to the workpiece enhances the kinetics of electrochemical reactions and hence enables the localisation of dissolution . As the temperature increases, the conductivity of the electrolyte increases, allowing a higher current density while higher temperatures on the workpiece lower the activation energy for the chemical reaction .
Relative increase in VRR for LAJECM vs. JECM 
IEG = 2 mm
IEG= 5 mm
Cp = 10%
Cp = 20%
Cp = 10%
Cp = 20%
Building upon this previous work, De Silva et al. performed further analysis of the thermal effects of JECM with both modelling and experimentation . Comparatively, the same laser density was used as in the study by Pajak et al. , 47.5 W/mm2, but with a lower range of electrolyte concentration, 5–10% concentration against the previously used 10–20%. As found previously, stainless steel and titanium alloy saw improved surface finishes when using LAJECM but Hastelloy (nickel-based alloy) saw no change with the introduction of laser assistance, and contrary to previous findings, aluminium alloy saw a larger surface roughness value with the introduction of laser assistance. LAJECM facilitates the removal of brittle oxide layers improving machining on titanium, an oxide prone metal, while increasing VRR and precision . However, De Silva et al. introduced a concern with LAJECM, where the increase in surface temperature and electrolyte temperature from laser absorption can cause electrolyte boiling. This electrolyte boiling can decrease electrolyte conductivity, because of machining stoppage and potential sparking.
Malik performed further experimental studies into LAJECM on Inconel 718 . Again, it was found there was a 29.7% increase in MRR with the introduction of laser assistance, and a 33.2% decrease in taper at optimal parameters.
Zhang et al.  proposed a novel hybrid process of laser drilling assisted with jet electrochemical machining in an experimental study, which was followed by a modelling and experimental study into the same process . Unlike the previous studies with the combined processes, these investigations aimed to maintain the laser drilling as the main material removal process with JECM as a secondary process. Recast and splatter are a major issue when producing holes with laser drilling; however, the introduction of JECM as a secondary process effectively reduces the recast and splatter at the cost an annular overcut at the entrance of the hole and a reduction in efficiency of up to 50% compared with laser drilling in air in both the study by Zhang et al.  and Zhang and Xu .
4.2 Ultrasonic-, air- and abrasive-assisted Jet-ECM
Air-assisted Jet-ECM uses a jet of air expelled co-axially or at an angle to the electrolyte jet. The air jet gives momentum to the flow of electrolyte radially across the surface of the part, moving the hydraulic jump on the material surface beyond the machining zone , an issue arising with lower electrolyte flow rates . In doing so, the current density is localised to the machining area, with the aim to reduce over cut and stray machining  while helping to remove debris from the machined area.
Ultrasonic-assisted Jet-ECM is a process in which ultrasonic vibrations are applied to the system via direct vibration of the tool or workbed , or via a separate ultrasonic emitter providing waves to the machining area [37, 46]. The aim of ultrasonic assistance is to enhance the reaction in the machining zone by aiding the removal of the reaction products . The ultrasonic assistance can also aid the breakdown of the passive layer on a material surface which prevents machining .
Abrasive-assisted Jet-ECM is a hybrid process that takes inspiration from water jet cutting, by adding abrasive particles to the jet of electrolyte. The aim of the hybrid process is to combine mechanical abrasion of the workpiece surface and passive layers with the electrochemical process for combined material removal mechanisms [49, 50].
In 2008, Hackert et al. used an additional jet of compressed air to remove the electrolyte film enclosing the nozzle caused by surface tension, and thus reducing the possible working gap . In the experiment, the air nozzle was not co-axial to the jet direction, but when machining pits, the stray machining was dramatically reduced. With this reduction, sharper edges were also produced in grooved channels, atypical for Jet-ECM processes . Later, Kai et al. used a co-axial air jet to produce a thin film on the workpiece surface at low electrolyte flow rates, which when unassisted do not produce a film flow . It was found the maximum depth of machined holes increased from 120 to 180 μ m with the use of air-assistance. Goel and Pandey performed a study into the effect of air-assisted Jet-ECM on MRR and hole taper  followed by a more in-depth performance evaluation of the process . It was found the taper of the hole increases with increased air pressure due to the reduction in stray machining  and localization of current density  while reducing the chance of sparking.
Goel and Pandey studied the effect of ultrasonic assistance alongside their experiments on air-assisted JECM  as well as in a following study . Goel and Pandey fabricated an attachment of consisting of a piezoelectric transducer at 20 kHz frequency, ultrasonic processor and ultrasonic horn . The aims of the ultrasonic assistance were to aid removal of the reaction products from the machining area and thus enhance the electrochemical reactions. It was found that the MRR increases up to 40% with the use of ultrasonic assistance and produce holes of less taper . Mitchell-Smith and Clare  studied the effect of ultrasonic assistance on removing the passive layer on titanium alloys during Jet-ECM. Whereas Goel and Pandey used acid electrolyte in the 2016 and 2017 studies, proven to aid the removal of passive layers , Mitchell-Smith and Clare claim this should be avoided as it creates a health and safety risk . Mitchell-Smith and Clare found the use of ultrasonic assistance enhanced the aspect ratio of the grooves due to passivation breakdown, increased depth and reduced passivation layer formation during machining by 23% . However, this study only used a single excitation frequency, and further work into frequency response is required.
Liu et al. also aimed to machine tungsten carbide with sodium chloride abrasive slurry electrolyte , compared with the mixed sodium chloride/sodium nitrate electrolyte used previously . Due to the material hardness, abrasive jet machining was unable to machine tungsten carbide with aluminium oxide particles, while Jet-ECM using non-abrasive sodium chloride electrolyte also proved to be ineffective due to the inability to breakdown the oxide layer , as previously found by Hackert-Oschätzchen et al. . The combined process allowed the machining of tungsten carbide due to the removal of the oxide layer using the abrasive particles followed by the dissolution of the unoxidized tungsten.
5 Conclusions and research challenges
Working gap has an effect on resistance, and therefore machined geometries. Larger gaps decrease MRR and surface roughness . A too small working gap does not allow the formation of a jet and hydraulic jump and hinders machining .
Surface roughness increases with reduced electrolyte concentration  on stainless steel with sodium nitrate solution.
MRR increases with increased electrolyte concentration, on stainless-steel samples using sodium nitrate electrolyte .
Use of a pulsed DC current improves the surface finish on stainless-steel samples with sodium nitrate electrolyte, but reduces MRR. 
Bipolar current increases the MRR rate with the same surface roughness value of a DC current, but erodes the tool .
All experiments studied used cylindrical nozzles varying from 0.05 mm diameter  to 2 mm diameter , aside from two studies where ‘letterbox’ nozzles were used for turning applications [13, 28]. In turning applications, the use of Jet-ECM was successful, producing high aspect ratios in turned rods, allowing larger areas to be machined than using a cylindrical nozzle. Jet-ECM has been proven to be able to produce complex 3D geometries in pitting, grooving and turning applications [1, 10, 13, 24] and the development is promising.
Changes to the nozzle geometries have been shown to alter the machined profiles, with the ability to produce more complex structures with nozzle combinations [31, 34]. Changing the angle of address of the nozzles can significantly enhance the precision of cuts  as well as increasing the depth of cuts .
When machining tungsten carbide alloys [20, 24, 28], the process raised more issues than when machining stainless-steel samples. When machining with pH-neutral electrolytes (NaNO3 and NaCl), oxide layer growth prevented machining. This was overcome by adding sodium hydroxide to the electrolyte to breakdown the tungsten oxide layer , or by using the NaOH produced naturally on the cathode surface during the Jet-ECM process. When using a ceramic nozzle and a DC current, the NaOH was mixed into the electrolyte, but resulted in less accurate machining . Alternatively, using an AC current produced NaOH on the workpiece when the current was reversed, allowing a breakdown of the tungsten oxide layer, but producing tool wear which could be reduced with the use of a ceramic nozzle .
When machining an aluminium matrix composite, Hackert-Oschätzchen (2016) found sodium nitrate electrolyte caused a passivating effect, while sodium chloride electrolyte, of equal conductivity produced pits with twice the depth with the same machining parameters. For titanium alloys [29, 30], sodium chloride produced a better pit depth, MRR and surface finish than bromide, nitrate and fluoride counterparts, partly due to the production of titanium chlorides that are hydrolysed and leaves no oxide layer when machining.
Iodide-doped electrolytes have been shown to increase precision  and dimensional accuracy  as well as improved surface finish in some cases over neutral electrolytes such as sodium chloride . Combinations of electrolytes can be used to further improve the Jet-ECM process .
More recent studies have developed hybrid processes involving Jet-ECM, namely laser-assisted, ultrasonic-assisted, air-assisted and abrasive-assisted hybrid processes. The use of laser assistance tends to improve the conductivity in electrolyte and material and localisation of the reaction at the risk of electrolyte boiling . It was in agreement throughout the studies that laser assistance increases the material removal rate compared with standard Jet-ECM [38, 39, 41, 42], especially at lower currents and electrolyte concentrations  as well as improving hole taper [6, 38, 39, 42]. The effect on roughness was material dependant  and in some cases, the laser assistance caused a larger overcut .
Air-assisted Jet-ECM can produce a lower working gap , while producing the thin film required for Jet-ECM when used co-axially with the electrolyte jet . The hybrid process was also shown to improve machining depth  while improving taper [37, 46, 51] through the reduction of stray machining, and producing sharper edges .
The introduction of ultrasonic assistance as a hybrid process again showed improvements over standard Jet-ECM. Material removal rate and taper were improved with the introduction of ultrasonic assistance on copper and stainless steel through as the ultrasonic vibrations aided the transport of reaction products from the reaction area [37, 48], with MRR improving by up to 40%. Mitchell-Smith and Clare also showed the useful nature of ultrasonic assistance in removing the passivation layer on titanium alloys  which was previously difficult with standard Jet-ECM.
The final hybrid process, combining abrasive particles within the electrolyte, also improved MRR over standard ECM  while improving surface roughness of machined areas, especially with a higher concentration of abrasive particles. Similarly to that found with ultrasonic assistance, slurry jet machining helps overcome passivation layers in tungsten carbide, allowing machining through the hybrid process that was not possible with either abrasive water jet machining or standard Jet-ECM .
This paper has described the experimental work performed in Jet-ECM and related hybrid technologies. Although research has accelerated from 2005 onwards, the picture of the process is not completely clear nor is it completely understood. More work still needs to be done in all aspects of the process, including a wider range of materials and electrolytes. The hybrid technologies outlined in this review also show good promise at early stages of research, but also require a larger amount of understanding to move the technology further towards being a fully understood and controlled technology. More recent studies have shown major improvements to system control and machining precision [4, 17, 31, 32, 35] but further developments are still required.
Jet-ECM requires an electrically conductive workpiece, and therefore removes the vast majority of non-metallic materials, vastly limiting the range of possible applications for machining.
The technology requires low transitional feed rates for material removal, in general less than 2 mm/s, which is more time consuming compared with laser technology or traditional manufacturing methods while producing lower material removal rates. Although nozzle design has aided the ability to machine a larger area [13, 28], applications for machining areas in the centimetre range have not been widely attempted.
Although assistive technologies such as laser assistance have been shown to improve the material removal rate, accuracy and surface roughness, the setups are more complex than those of non-assisted counterparts and are thought to reduce the cost-effectiveness of the technology.
The nature of the process produces naturally rounded edges as well as tapered holes and geometries, and is not suitable to produce geometries 90∘ to the top machined surface. In addition, the high aspect ratios achieved in EDM (ratios up to 15) are not achievable in Jet-ECM nor are the accuracies in the range of 1 μ m achieved in EDM possible with Jet-ECM, with accuracies of around 5 μ m  with overcuts commonly found.
Only external component surfaces of metallic parts have been machined, and within that only top surfaces, limiting the features Jet-ECM can process; however with developments in the angle of address , a wider range of features should be accessible for machining with further work.
Moving forward, a combination of experimental and modelling work must be performed to move away from a prediction of machined geometries based around machining trials and towards a predictable machining outcome based around parameters. The challenge is understanding the effect of each process variable, their relationships to other variables, and knowing these effects on a wider range of materials than is currently known. This challenge will be increased with the introduction of hybrid technologies, adding further unknown variables to the process.
Applications mentioned in research have been minimal, with the use of the technology leaning towards biomedical applications  with several studies being performed on biomedical-type materials. Further applications for the technology need to be found and developed, with the Jet-ECM process being tested as a manufacturing technique and assessed for industrial use. In doing so, the range of geometries and materials currently capable of being processing need to be developed and increased.
This study was financially supported and sponsored by Blueacre Technology, as well as by the DTP scholarship through ESPRC.
- 1.Natsu W, Ikeda T, Kunieda M (2007) Generating complicated surface with electrolyte jet machining. Precis Eng 31(1):33–39. https://doi.org/10.1016/j.precisioneng.2006.02.004, book 1CrossRefGoogle Scholar
- 6.Pajak P T, Desilva A K M, Harrison D K, McGeough J A (2006) Precision and efficiency of laser assisted jet electrochemical machining. Precis Eng 30(3):288–298. https://doi.org/10.1016/j.precisioneng.2005.09.006 CrossRefGoogle Scholar
- 7.Wang M, Bao Z, Qiu G, Xu X (2017) Fabrication of micro-dimple arrays by AS-EMM and EMM. The International Journal of Advanced Manufacturing Technology https://doi.org/10.1007/s00170-017-0538-0
- 12.Kunieda M (1993) Influence of micro indents formed by electro-chemical jet machining on rolling bearing fatigue life. ASME PED 64:693–699Google Scholar
- 14.Schubert A, Hackert-Oschätzchen M, Meichsner G, Zinecker M, Martin A (2011) Evaluation of the influence of the electric potential in jet electrochemical machining. In: 7th International Symposium on Electrochemical Machining Technology (INSECT). book 1, vol 1, pp 47–54Google Scholar
- 24.Hackert-Oschätzchen M, Martin A, Meichsner G, Zinecker M, Schubert A (2013) Microstructuring of carbide metals applying jet electrochemical machining. Precis Eng 37(3):621–634. https://doi.org/10.1016/j.precisioneng.2013.01.007 CrossRefGoogle Scholar
- 25.Schubert N, Schneider M, Michaelis A (2011) Investigation of anodic dissolution of cobalt in alkaline solution. In: Proceedings of the 7th International Symposium on Electrochemical Machining Technology, vol 1, pp 31–37Google Scholar
- 31.Clare AT, Speidel A, Bisterov I, Jackson-Crisp A, Mitchell-Smith J (2018) Precision enhanced electrochemical jet processing. CIRP Annals, https://doi.org/10.1016/j.cirp.2018.04.086
- 38.Malik A, Manna A (2018) Investigation on the laser-assisted jet electrochemical machining process for improvement in machining performance. The International Journal of Advanced Manufacturing Technology https://doi.org/10.1007/s00170-018-1846-8
- 46.Goel H, Pandey P (2015) Experimental investigations into micro-drilling using air assisted jet electrochemical machiningGoogle Scholar
- 50.Liu Z, Nouraei H, Spelt J K, Papini M (2015) Electrochemical slurry jet micro-machining of tungsten carbide with a sodium chloride solution. Precis Eng 40:189–198. https://doi.org/10.1016/j.precisioneng.2014.11.009 CrossRefGoogle Scholar
- 51.Hackert M, Meichsner G, Schubert A (2008) Generating micro geometries with air assisted jet electrochemical machining. European Society for Precision Engineering and Nanotechnology, EUSPEN 2008(2):420–424Google Scholar
- 52.Hackert-Oschätzchen M, Meichsner G, Zinecker M, Martin A, Schubert A (2012) Micro machining with continuous electrolytic free jet. Precis Eng 36(4):612–619. https://doi.org/10.1016/j.precisioneng.2012.05.003, book 1CrossRefGoogle Scholar
Open Access This article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.